Download presentation

Presentation is loading. Please wait.

Published byDemarcus Letter Modified over 2 years ago

1
Viscous Deformation of a Fused Quartz Tube Caused by Furnace Malfunction: Modeling and Analysis Sunny Sue Wicks Stephen Alan Steiner III Massachusetts Institute of Technology Fall 2007 ES240 Final Project

2
Introduction Electric clamshell or “tube” furnaces are commonly used in materials science labs for chemical vapor deposition, annealing Furnaces typically have three independently-controllable electric heating coils or “zones” rated for 1200°C service A fused quartz tube is used often used to contain the process reaction

3
One Dark And Stormy Night at MIT... An 1100°C process was being run when thermocouples in Zones 1 and 2 broke - apparently a thermocouple was in direct contact with a heating coil The temperature controller went to full duty cycle and Zone 1 went on thermal runaway (1200°C or greater) Zones 2 and 3 remained on but it’s not certain how hot After four hours or so, the fused quartz tube was found draping out of the left side of the furnace Before process After process

4
Zone 1Zone 2Zone 3 77.15 cm 7.62 cm 20.64 cm Zone 1Zone 2Zone 3 Furnace Dimensions 28.26 cm 32.23 cm 366.98 g 18.02 cm Φ tc = 0.238 cm Center of dimple from thermocouple on deformed tube is 0.8220 cm from Tag 5 Positioning in Furnace 5.3848 cm OD 4.9610 cm ID 137.80 cm Tube Diameters and Lengths Material is fused quartz 5.4420 cm OD 140.02 cm Actual Measurements

5
13 12 1110 9 8 Relative Deflection Measurements Plot of Deflection Data, Rotated 5° Image analysis was used to determine deflections relative to a new fused quartz tube

6
Questions What temperature did Zone 1 likely reach? How and why did the fused quartz tube deform the way it did? Why did the tube cross section pinch near the point where it inflected?

7
Projected Zone 1 Projected Zone 1 Temperature Temperature Profile Temperature readings peaked, temperature controller began to malfunction Thermocouples failed

8
Methodology Analytical Model (Simple Beam Theory) Finite Element Modeling (Two- Layer Viscoplastic Model in ABAQUS) Empirical Analysis (Deflection Data, Shape Trends)

9
Temperature is significantly below T g so material is elastic and brittle Circular cross-section of the tube does not deform during bending Tube length is much greater than tube diameter Loading and deflection occur in vertical direction only Small deflections Simple Beam Theory Model: Assumptions

10
Simple Beam Theory Pinned in two locations Distributed load from weight of tube End loads from weight of aluminum endcaps 0.32 m0.77 m 0.28 m P = 14.16 N/m Analytical Model: Derivations F = 3.6 N R 1 = 3.8 N R 2 = 3.4 N

11
∑ F = 0 ∑ M = 0 This is true for any part of the beam : F M(x) S(x) -0.4-0.200.20.40.60.811.2 -4 -3 -2 0 1 2 3 4 x, [m] Shear and Moment Quartz Tube at Ambient Temperature S(x), [N] M(x), [N*m] Analytical Model: Simple Beam Theory

12
-0.4-0.200.20.40.60.811.2 0 1 2 3 x 10 5 x, [m] σ xx in Pure Elastic Case -0.4-0.200.20.40.60.811.2 -3 -2 0 1 x 10 -5 x, [m] Deflection, [m] Deflection in Pure Elastic Case σ xx, [Pa]

13
Viscoelastic: Deformation is completely reversible Viscoplastic: Plastic behavior comes into play after the yield stress is reached Viscous: Strain rate directly proportional to stress, regardless of stress magnitude; a subcategory of creep For Fused Quartz: Strain Point ( η = 10 13.5 ): 1120°C Annealing Point ( η = 10 12 ): 1215°C Possible Deformation Pathways Viscosity Equation: Glasses behave like “frozen liquids”

14
In beam bending, deflection results from the large σ xx, so we consider a uniaxial stress case =2*strain rate Definition of Viscosity From Class: This means: For uniaxial stress For pure shear stress Viscous Behavior

15
t = 0, ε = ε elastic t > 0, Furnace runs away, ‘Cool’ regions remain elastic, ε = ε elastic Hot region starts to viscously flow, ε = ε elastic + ε plastic F = 3.6 N R 1 = 3.8 N R 2 = 3.4 N 0.32 m 0.77 m 0.28 m Modifying Simple Beam Theory to Include Viscosity in Hot Zone 1200°C+ Region

16
Where, σ xx = f(t), from simple beam theory η = f (T(t)), from a given temperature profile, and the derived viscosity equation Discretized ε xx final can be fitted with a second order polynomial Numerical integration ε xx i+1 = σ xx / η * ∆t + ε xx i We now have all the tools to take a given temperature profile and estimate the tube deflection Viscous Strain

17
Contributing Uncertainties: 1200°C is the rated maximum temperature max - the maximum temperature 100% duty cycle is likely higher Model only allows concave down curvature while tube exhibits some concave up behavior in Zone 2 Temperature surrounding Zone 1 (in ceramic collar and in Zone 2) is uncertain Tube Deflection at Temperature of 1200 ° C in Zone 1 Deflection Results from Model

18
Deflection Results from Model: Higher Temperatures Zone 1 TemperatureMax Deflection, LeftMax Deflection, Top 1200°C-0.22 cm0.11 cm 1250-1.4 cm0.60 cm 1275-3.0 cm1.4 cm 1300-6.9 cm3.3 cm Actual-9.7 cm3.4 cm -0.4-0.200.20.40.60.811.2 -0.08 -0.06 -0.04 -0.02 0 0.02 0.04 x, [m] deflection, [m] Deflection at 1300 ° C

19
Finite Element Model Run in ABAQUS 6.7.1 Objectives were to get a functional model and to observe phenomena not captured by simple beam theory Used two approaches: Standard 3D deformable solid with a higher compliance in Zone 1 (to identify behaviors due to large deflections) Full coupled temperature-displacement model (to simulate viscous flow) 3 2 1

20
3D Deformable Solid Defined Zone 1 region with a Young’s modulus of 2 GPa, rest of tube with 70 GPa Observed similar shape trend as beam theory, but deflections were four orders of magnitude off Suggests concave section in Zone 2 results from plasticity

21
Coupled Temperature-Displacement ABAQUS models viscous flow using a two-layer viscoplasticity model - requires defining elastic, plastic, and viscous components (viscous A=5.7836x10 -13, n=1, m=0, f=0.99999) Must define thermal conductivity and specific heat Used a C3D8T element type Divided tube into seven regions, assigned temperatures as “Initial Conditions” Boundary conditions: U1, U2, U3, UR2, and UR3 restricted where tube contacted edge of ceramic collars Modeled Zone 1 at 1200°C-1300°C for 4-40 hrs. KpKp KvKv η, m σγσγ H’

22
Coupled Temperature-Displacement 1200°C, 4 hrs. Shape trend was different from simple beam theory/actual data Similar deflections only observed after 40 hrs., significantly longer than actual experiment time Zone 1MaxMax TemperatureTimeDeflection, LeftDeflection, Top 1200°C4 h-0.22 cm0.11 cm 120040-5.12.2 13004-0.220.11 Actual4-9.73.4

23
Conclusions General bending behavior captured with simple beam theory and finite element models The deformations resulting from the viscous behavior in the fused quartz are significantly impacted by temperature, time Concave dip in Zone 2 region implies some information is missing regarding the temperature profile in this zone Temperature was likely hotter than 1200°C Pinching at the top of the tube is not a direct result from tube bending or from viscous flow - likely because of impeded deflection against thermocouple Accurate viscous deformations are difficult to model in ABAQUS

Similar presentations

© 2017 SlidePlayer.com Inc.

All rights reserved.

Ads by Google